Growth and Characterisation of
Gold-seeded Indium Gallium Arsenide
Nanowires for Optoelectronic Applications
A thesis submitted for the degree of
Doctor of Philosophy
The Australian National University
Amira Saryati Ameruddin
This thesis, to the best of my knowledge and belief, does not contain any results
previously published by another person or submitted for a degree or diploma at any
university except where due reference is made in the text.
Amira S. Ameruddin
Department of Electronic Materials Engineering,
Research School of Physics and Engineering,
College of Physical and Mathematical Sciences,
The Australian National University,
First and foremost, Alhamdulillah (all praise for Allah), for the strength He lends, the blessings and the knowledge gained throughout my journey of completing this thesis.
I would like to express my gratitude to my supervisors, Prof. Hark Hoe Tan, Prof. Chennupati Jagadish, Dr. Philippe Caroff and Assoc. Prof. Jennifer Wong-Leung for their guidance, support and knowledge shared along the whole time of my PhD. I thank Prof. Jagadish for his great support, his insight on the research and wise advices he had given. He is someone I look up to with respect and aspire to. I am extremely grateful to have Hoe as my main supervisor who has guided me in all aspects of research throughout the whole journey. He always has his door open for discussion, which had helped me immensely. I am always in awe for his quick, smart responses to questions and problems I had. I would like to especially thank Philippe, for his tremendous help with research aspects and sharing his ideas; he is like a knowledge bank to me. His passion for research is inspiring and I believe his presence has made my PhD journey more pleasant and enjoyable. My acknowledgement is also for Jenny, for her guidance in TEM, especially during those few months learning to look at nanowires under TEM. I remembered the struggle I had trying to get to the zone axis and the only thing that keeps me going was her words “It will get to you like driving a car”. Indeed it did. I am also thankful for many discussions we had on the TEM and EDX analyses.
Dr. Steffen Breuer, Dr. Patrick Parkinson and Dr. Hannah Joyce, former staff and student, of the group are included in this list of acknowledgements. We had several discussions during my early PhD years regarding my research, which had helped me and guided me during those early days. I would like to thank Dr. Yanan Guo and Dr. Fan Wang for their help and support with experimental work during the time they were at the department.
I would like to thank my fellow colleagues; Aruni Fonseka for her supports and her guidance in almost all of the experimental and writing involved during my PhD, Jenny Jiang for the time she spent teaching me how to make nanowire cross-sections; Xiaoming Yuan, Qian Gao, Kun Peng, Dhruv Saxena and Bijun Zhao for sharing their knowledge and discussing our progress together. Other students in the group are also acknowledged for their presence, supports and their insight on research. Other staff members including Assoc. Prof. Lan Fu, Dr. Sudha Mokkapati, Dr. Shagufta Naureen, Dr. Ziyuan Li are also acknowledged for numerous occasion and supports.
Not to be forgotten, all of the technical staffs involved are also gratefully acknowledged. Dr. Mykhaylo and Jason for their help with MOCVD; David Llewlyn, Dr. Animesh Basek, Dr. Frank Brink, Dr. Hua Chen, Joanne Lee, Dr. Felipe Kramer for their help with microscopy; and other ANFF staff member for their help with equipment I used throughout my PhD. I am thankful to Scott Yates and Julie Arnold. They have been helpful in taking care all of the administrative work involved during my years in EME and have been so helpful on many occasions. Karen Nulty and Liudmilla Mangos who have assisted me with the administrative part of the graduate office are also acknowledged. Apart from them, I would also like to acknowledge the scholarship from the Malaysian government and Universiti Tun Hussein Onn Malaysia and the people involved with the scholarship administrative work.
Special friends like Aruni Fonseka, Allina Nadzri, Huda Alkhaldi, who has not only shared their time discussing work but also have shared laughs and stress moments together deserve a special acknowledgement. I am greatly thankful for their friendship and support. My thanks also goes to people behind the scene, friends whom I spend time with outside working hours, who have listened, support and keep me motivated with my studies.
1. Ameruddin A. S , Caroff P., Tan H. H., Jagadish C., Dubrovskii V. G. “
Understanding the growth and composition evolution of gold-seeded ternary InGaAs nanowires” Nanoscale, 7, pp. 16266 – 16272, 2015
2. Ameruddin A. S., Fonseka H. A., Caroff P., Wong-Leung J., Op het Veld R. L.M., Boland J. L., Johnston M. B., Tan H. H., Jagadish C. “InxGa1-xAs nanowires with uniform composition, pure wurtzite crystal phase and taper-free morphology” Nanotechnology, 26, p. 205604, 2015
3. Fonseka H. A., Caroff P., Wong-Leung J., Ameruddin A. S., Tan H. H., Jagadish C., “Nanowires Grown on InP (100): Growth Directions, Facets, Crystal Structures, and Relative Yield Control” ACS Nano, 8 (7), pp. 6945–6954, 2014
4. Ameruddin A.S., Tan H. H., Fonseka H. A., Gao Q., Wong-Leung J., Parkinson P., Breuer S. and Jagadish C. “Influence of growth temperature and V/III ratio on growth of Au-assisted InxGa1-xAs nanowires” COMMAD 2012
5. Ameruddin A.S., Caroff P., Tan H. H., Wong-Leung J., and Jagadish C. “Growth and bandgap tunability of strained InGaAs/InGaP core-shell nanowires” in
preparation, to be to be submitted.
Semiconductor nanowires have been the spotlight of the last two decades owing to their novel properties and quantum confinement properties with their unique rod-like structure. In particular, III-V semiconductor nanowires have been shown as promising candidates to serve as building blocks in electronic and optoelectronic devices such as transistors, lasers, light emitting diodes, photodiodes and solar cells. Among the III-V semiconductors, ternary III-V alloy semiconductors such as InxGa1-xAs have the advantage of tunable bandgap by varying their alloy composition. InxGa1-xAs has a bandgap that is tunable in between GaAs (870 nm) to InAs (3500 nm) covering the important wavelengths used in optical telecommunication systems and sensing in near infra-red region. Therefore, it is essential to gain an understanding and control of ternary nanowires in terms of their composition, crystal structure and morphology prior to incorporating them in device applications.
This thesis presents a progressive advancement of Au-seeded InxGa1-xAs nanowire growth by metal-organic vapour phase epitaxy (MOVPE), towards achieving highly uniform composition, morphology and pure crystal phase. Several techniques have been employed to investigate the nanowire properties. Scanning and transmission electron microscopy, atomic force microscopy, X-ray diffraction (XRD) and energy dispersive X-ray spectroscopy (EDX) have been used for structural and compositional analysis, while photoluminescence (PL) has been used to provide insight into their optical properties.
Homogenous composition along and across the InxGa1-xAs nanowires can also be achieved at relatively high temperatures with tunable phase. Detailed TEM analysis in combination with the EDX show that the crystal phase is dependent on the V/III ratio, and correlates with the Ga incorporation rate in the nanowire. The composition and crystal phase is tunable with V/III ratio and Au seed particle size. In particular, pure wurtzite (WZ) phase, uniform and taper-free nanowires are obtained with a combination of relatively high growth temperature, low V/III ratio and small diameter Au seed particle. The optimized pure WZ phase nanowires capped with InP show luminescence properties around 1.54 μm, a wavelength region of importance to the optical fibre telecommunications.
Understanding the growth evolution of InxGa1-xAs nanowires is improved by developing a model based on a nucleation kinetics approach. The modelling correlates well with the experimental results revealing the key factors governing the composition and growth rate of InxGa1-xAs nanowires. Small diameters and low V/III ratios result in As-limited regime VLS growth while for larger diameter nanowires and higher V/III ratios, the growth is group III limited. The In content in the nanowires is noticeably larger than that in the vapour phase and this is found to be highly related to the high In diffusivity at higher temperatures and low cracking efficiency of the Ga precursor at lower temperatures.
Finally, tunable emission wavelengths of InxGa1-xAs /InGaP core-shell structures within the range of 1100 – 1420 nm are achieved by tuning the shell thickness. The growth of the complex ternary/ternary system is studied using TEM and EDX analyses, revealing some challenges in the growth of the ternary shell on the pure phase WZ and the defective ZB phase InxGa1-xAs nanowires. Despite the challenges, the emission from the InxGa1-xAs core can be tuned by changing the shell thickness, indicating a strain related blue-shifting of the InxGa1-xAs bandgap.
List of Acronyms and Symbols ...
List of Figures ...
List of Tables ...
Chapter 1 : Introduction
Ternary InxGa1-xAs semiconductor material………..
Ternary III-V semiconductor nanowires……….
1.2.1 Growth of ternary III-V nanowires………..
188.8.131.52 VLS growth of ternary III-V nanowires……….
184.108.40.206 Particle/droplet free growth of InGaAs nanowires..
1.2.2 Application of ternary III-V nanowires in devices….……...
1.2.3 Ternary III-V nanowires review summary………
1.3 Thesis synopsis………
Chapter 2: Basic concepts
Semiconductor nanowire heterostructures………..
Semiconductor nanowire growth………
2.3.1 Nucleation theory………..
2.3.2 Phase diagram……….
2.3.3 Mass transport………
2.3.4 Growth of nanowire heterostructures………...
2.4 III-V nanowire crystal structure………...
Chapter 3: Experimental Techniques
3.2 Metal-organic Vapour Phase Epitaxy (MOVPE)………..
3.2.1 Basic principles of MOVPE………..
3.2.2 Components of MOVPE……….
220.127.116.11 Gas delivery system………...
18.104.22.168 Reactor System……….
22.214.171.124 Exhaust System………
3.2.3 Au-assisted InGaAs nanowire growth by MOVPE…………
3.3 Scanning Electron Microscopy (SEM)………...
3.3.1 Basic principle of SEM………...
3.3.2 Components of SEM………...
126.96.36.199 Electron guns………...
188.8.131.52 Electromagnetic coil lenses………..
184.108.40.206 Vacuum system………...
3.3.3 Determining the parameters of nanowires using SEM
3.4 Transmission Electron Microscopy (TEM) ………...
3.4.1 Basic principle of TEM………...
3.4.2 Components of TEM………...
220.127.116.11 Nanowire specimen preparation for TEM…………...
3.5 Scanning Transmission Electron Microscopy (STEM) and
Energy Dispersive X-ray (EDX) Spectroscopy……….
3.5.2 EDX spectroscopy………...……….
3.5.3 Qualitative and quantitative EDX analysis………
3.6 Photoluminescence (PL) ………...
3.6.1 Basic principle of PL spectroscopy………
3.6.2 Components of PL setup………...
Chapter 4: Pure zinc-blende phase high In Inx
grown by two-temperature growth method
4.2 Experimental method……….
4.3 Two-temperature growth method for crystal phase purity……
4.4 Effect of flow ratio of precursors……….
Chapter 5: Controlling the phase and composition tunability of
5.2 Experimental method………..
5.3 Effect of growth temperature and V/III on morphology and
5.4 Effect of growth temperature and V/III ratio on crystal
structure and composition………...
5.5 Effect of Au-seed particle size on morphology, crystal
structure and composition………...
5.6 Optical properties of WZ InxGa1-xAs /InP nanowire core-shell
Chapter 6: Towards understanding of Au-seeded Inx
nanowire growth evolutions
6.2 Scientific hypotheses and assumptions for the model………
6.2.1 General context of the growth model………...
6.2.2 Composition of Au alloy particle and nanowire solid……
6.2.3 Nucleation model………..
6.2.4 Diffusion transport………..
18.104.22.168 Diffusion transport of group III species……….
22.214.171.124 Diffusion transport of As species………
126.96.36.199 Model derivation for InxGa1-xAs nanowire
composition and growth rate………..
6.3 Relationship between the model and the experimental results
6.3.1 InxGa1-xAs nanowire composition………...
188.8.131.52 InxGa1-xAs nanowire composition and growth
rate versus Au seed diameter……….
184.108.40.206 InxGa1-xAs nanowire composition and growth
rate versus nominal V/III ratio………..
220.127.116.11 InxGa1-xAs nanowire composition and growth
rate versus nominal V/III ratio………..
6.4 Limitation and future improvement………..
6.4.2 Radial growth………..
6.4.3 Crystal phase………...
Chapter 7: Bandgap tunability of InGaAs/InGaP nanowire
7.2 Experimental method………..
7.3 Morphology and structural properties of WZ and ZB phase
InGaAs/InGaP core-shell heterostructures………
7.3.1 Morphology and structural properties of WZ
InGaAs/InGaP core-shell heterostructures………
7.3.2 Morphology and structural properties of ZB
InGaAs/InGaP core-shell heterostructures………
7.4 Optical properties of InGaAs/InGaP core-shell
7.4.1 Photoluminescence of WZ In0.60Ga0.40As/In0.60Ga0.40P
7.4.2 Optical properties of ZB In0.55Ga0.45As/In0.60Ga0.40P
Chapter 8: Summary and future outlook
8.2 Future outlook………..
List of acronyms and common symbol
A.U arbitrary units
BSE back scattered electrons
DOS density of states
EDX energy dispersive X-ray spectroscopy
FESEM field-emission scanning electron microscopy
FWHM full width at half maximum
HAADF high angle annular dark field
MOVPE metal organic vapour phase epitaxy
QD quantum dot
QW quantum well
QWR quantum wire
QWT quantum well tube
RT room temperature
SAED selected area diffraction pattern
SE secondary electron
SEM scanning electron microscopy
STEM scanning transmission electron microscopy
TEM transmission electron microscopy
List of Figures
1.1 Band gap versus lattice constant diagram for the common semiconductor
2.1 Schematic diagrams of nanowire axial and radial heterostructures……… 21
2.2 Schematic diagrams of quantum dots and quantum well tube in a free-standing nanowire………... 21
2.3 Quantum wire along the nanowire length and quantum dot in the corners of the nanowire side facets………... 22
2.4 Bandstructure of InAs/GaAs core-shell nanowires……… 23
2.5 Schematic of VLS growth of Si nanowires………. 24
2.6 Schematic of selective-area growth of nanowires……….. 25
2.7 Schematic of VLS growth with the supersaturation relevant to the three phase system……….……….. 26
2.8 Ternary phase diagram for Au-Ga-As and Au-In-As………... 27
2.9 Calculated monovariant lines of the Au–In–Ga system along with isothermal liquidus projections……….……… 28
2.10 Stacking sequence of the crystal phase for zinc-blende and wurtzite structure.……….……….………... 31
2.11 TEM images with the stacking sequences……….. 32
3.1 Schematic representation of examples of processes and mass transport that can occur during epitaxial growth………. 44
3.2 Schematic diagrams of major components in a typical MOVPE system…………. 45
3.4 Growth temperatures versus time for a typical nanowire growth……… 49
3.5 Electron-sample interaction……….………. 50
3.6 Schematic of a typical SEM showing the main components………... 51
3.7 Schematic of Everhart-Thornley detector……… 52
3.8 Evaluation of nanowire dimensions from tilted SEM image and facet determination from top view SEM image……….. 53
3.9 Bragg scattering process………. 54
3.10 TEM photo and its schematic showing the internal structure……….. 56
3.11 The ultramicrotome slicing technique………. 58
3.12 The process of Bremsstrahlung and characteristic x-rays emission………….... 59
3.13 Representative of an EDX spectrum of an Au particle……… 60
3.14 Graph of k values for GaAs and InAs nanowires versus diameter……….. 62
3.15 The basic processes involved in photoluminescence………..……... 63
3.16 Schematic of a typical PL setup……… 64
4.1 FESEM image, TEM and EDX spot analysis of InxGa1-xAs nanowires grown at a (single) temperature of 450 °C………. 71
4.2 FESEM images of nanowires grown at various growth temperatures……… 72
4.3 EDX line scan for InxGa1-xAs nanowires grown at various growth temperatures……….………. 73
4.4 : TEM image of a nanowire grown with the two-temperature growth method at Tg = 375 ºC……….……….. 74
List of Figures
4.6. EDX line scan along the nanowire for the sample grown at Tg = 375 ⁰C with
Xv(In) = 0.10.……….………..……… 76 4.7 EDX-STEM cross-section maps of Ga, In and the overlay of In and Ga of a
nanowire grown with Xv(In) = 0.30 and 0.10………. 77
4.8 Average In molar fraction in the nanowire core versus TMIn molar fraction supplied in vapour……….……….. 78
5.1. FESEM images of nanowires grown at various growth temperatures and
V/III ratio of 40.0 and 2.4……….……….……….. 88
5.2 FESEM image, HRTEM and EDX cross-section map of nanowires grown at
growth temperature of 450 °C and a V/III ratio of 40.0………..………. 90
5.3 FESEM image, HRTEM and EDX cross-section map of nanowires grown at
growth temperature of 500 °C and a V/III ratio of 40.0………... 91
5.4 FESEM images, HRTEM and EDX line scan of nanowires grown at 500 °C
with increasing V/III ratio from 1.4 to 40.0………. 93
5.5 TEM and HRTEM image of the nanowire that was grown at 500 ºC and V/III
ratio of 2.4 for 30 minutes then V/III ratio of 86 for 10 minutes... 95
5.6 The average percentage of twinned bilayers and Ga molar fraction as
determined by the EDX, XGa against the V/III ratio……….. 96
5.7. EDX spectrum was taken at the middle of the nanowire Au-alloy particle for the sample grown at 500 °C and V/III ratio of 20.0………..….. 97
5.8. FESEM image, TEM and cross-sectional EDX of the 7 µm long almost
defect-free WZ InxGa1-xAs nanowire……….………….………... 98
5.9 FESEM image and TEM of nanowires grown at 500 °C with V/III ratio of 1.4
seeded with 10, 20, 30, 50 and 80 nm Au-particle size………. 100
5.10 The average percentage of twinned bilayers and Ga molar fraction, XGa
against the Au-seed particle……….……….. 101
5.11: HAADF image and EDX maps of composition distribution around the tip
area of the 80 nm Au-seeded nanowire……….. 102
5.12 SEM image, cross-sectional view HAADF and EDX analysis of InxGa
5.13 Photoluminescence spectra of ensemble of In0.65Ga0.35As nanowires and
In0.65Ga0.35As /InP core-shell heterostructure nanowires measured at 6 K …………. 104
6.1 Schematics of Au-assisted InxGa1-xAs nanowire growth by MOVPE
6.2 HAADF and EDX spot analysis of a nanowire grown with 50 nm Au alloy
6.3 Experimentally determined and model fitting of nanowire composition and
axial growth rate versus Au alloy particle diameter……….. 121
6.4 Experimentally determined and model fitting of nanowire composition and
axial growth rate versus V/III ratio……….. 122
6.5 Experimentally determined and model fitting of nanowire composition and
axial growth rate versus growth temperatures………... 123
7.1 FESEM images of 30 nm seeded bare InGaAs nanowire and InGaAs/InGaP
grown with 3:20, 8:00 and 40:00 InGaP shell growth time... 134
7.2 TEM, HRTEM and EDX spot analysis of 30 nm seeded InGaAs nanowire with
3:20 minutes InGaP shell………. 136
7.3 TEM, HRTEM and EDX map and spot analysis of 30 nm seeded InGaAs
nanowire with 8:00 minutes InGaP shell. ………. 137
7.4 HRTEM, HAADF and EDX map of symetric hexagonal cross-section and
truncated triangular cross-section……… 139
7.5 TEM, HRTEM and EDX spot analysis of 30 nm seeded InGaAs nanowire with
40:00 minutes InGaP shell. ……… 141
7.6 FESEM images of 50 nm seeded bare InGaAs nanowire and InGaAs/InGaP
grown with 3:20, 8:00 and 40:00 InGaP shell growth time... 141
7.7 TEM, HRTEM, EDX spot analysis and EDX cross-section map of 50 nm seeded
InGaAs nanowire with 8:00 minutes InGaP shell..………... 142
7.8 Normalized PL spectrum of 30 nm Au-seeded WZ phase
In0.60Ga0.40As/In0.60Ga0.40P with shell growth time of 8:00 and 40:00
List of Figures
7.9 Normalized PL spectrum of 50 nm Au-seeded ZB phase
In0.55Ga0.45As/In0.60Ga0.40P with shell growth time of 3:20, 8:00 and 40:00
8.1 FESEM image, TEM and EDX line scan of InGaAsP nanowire with nominal
List of Tables
7.1 Dependence of InGaP shell thicknesses with growth time for 30 nm
Au-seeded WZ nanowires………
7.2 Dependence of InGaP shell thicknesses with growth time for 50 nm
Au-seeded ZB nanowires….………
7.3 The PL peak position for the InGaAs/InGaP core-shell nanowires with
Nanowires, nanowhiskers, nanobelts or in general, 1-dimensional (1D) semiconductor nanostructures have been the subject of intense research in the past few decades since the first attempts at understanding their growth mechanism by Wagner and Ellis in the 1960’s and Givargizov in the 1970’s , . In the late 1990s, the research expanded significantly to include not only interest towards the understanding of fundamental nanowire growth, but also exploration of their electronic and optical properties as well as for device applications –. As part of the still expanding effort in the field of semiconductor nanowire research, this thesis is focused on trying to understand the fundamental nanowire mechanisms, especially of the ternary compound semiconductor, indium gallium arsenide (InGaAs or InxGa1-xAs). The study covered in the thesis provides insight into the foundation
1.1 Ternary Inx
As semiconductor material
InxGa1-xAs system is one of the most interesting III-V ternary alloy semiconductors because
of several key properties such as very high carrier mobility (µe=~10000 cm2V-1s-1, µh=~300
cm2V-1s-1) and a large range of direct bandgaps tunable between InAs and GaAs. For
example, InxGa1-xAs can be tuned to the telecommunication wavelengths range of 1.3 - 1.55
µm (0.80 - 0.95eV) and to an even longer wavelength (near infra-red, NIR) region for detection applications such those used in agriculture at 1.9 µm (0.65 eV) and in environmental monitoring .
Figure 1.1: Band gap versus lattice constant diagram for the common semiconductor
materials. Highlighted line represents InGaAs while the vertical line across InP shows the lattice matched condition of In0.53Ga0.47As to InP.
Figure 1.1 shows the common semiconductor bandgap versus lattice constant at room temperature, highlighting the line representing InxGa1-xAs alloys. As can be observed,
InxGa1-xAs bandgap can be tuned from ~0.35 to 1.424 eV and the lattice constant varies
The lattice constant of InxGa1-xAs given by Vergard’s Law is:
a = 6.0583 − 0.405 (1 − x) (1.1)
At room temperature (300 K) the dependency of the energy gap on the In content x can be calculated using an equation given by  as follows :
Eg(x) = 1.425 – (1.501) x + (2 0.436) x2 eV (1.2)
InxGa1-xAs can be lattice matched to InP by tuning the composition to In0.53Ga0.47As which is
highly desirable especially in growing 2-D structures where lattice-matching is required. However, in nanowire form, a higher level of strain can be accommodated thus InxGa1-xAs
can be combined together with many other materials such as AlxGa1-xAs, InxGa1-xP, InxGa
1-xAsyP1-y a nanowire heterostructure which can provide an extension to their tunability of
properties through bandgap engineering. Heterojunction is highly important in making semiconductor devices . The concept of nanowire heterostructures will be further discussed in chapter 2. InxGa1-xAs properties together with other advantages of nanowires as
shall be discussed later in chapter 2, makes InxGa1-xAs nanowires desirable for nanowire
devices. In the following section, a review on ternary III-V nanowire growth including InGaAs nanowires and their applications are presented.
1.2 Ternary III-V semiconductor nanowires
A wide range of semiconductor materials such as group IVs, III-Vs, II-Vs, oxides and II-Vs for nanowire growth have been investigated in the last decades , , , . In particular, III-V materials have been of great interest due to their outstanding properties , , , . Extensive efforts have been dedicated to synthesizing and optimizing III-V nanowires because of their demonstrated superior optoelectronic properties, but efforts have focused largely to date on binaries and their heterostructures. Ternary III-V alloys such as InxGa1-xAs,
InxGa1-xP, InAsxP1-x and GaAsxSb1-x on the other hand have not yet been explored as deeply as
the binary nanowires despite of their ability to access a larger controllable range of bandgaps, which in turn provides more room for tunability of their optical emission/absorption.
ternary nanowires suffer from intrinsic issues of composition inhomogeneity or variation over certain growth directions. Composition homogeneity is highly essential as a prerequisite to use III-V ternary nanowires in device applications. This is to avoid additional problems such as severe electron scattering , induced strain field or any other additional problem due to the alloy fluctuation in the crystal, such as alloy ordering affecting the bandgap of the material . In addition to homogeneity, having control over the composition range is important as to be able to provide the range of properties afforded by the appropriate choice of alloy composition.
Nevertheless, other common challenges encountered with many nanowires such as controlling the morphology and crystal structure of the nanowires are equally important and not avoidable for III-V ternary nanowires as shall be discussed later in this section. In fact, they are even more challenging as more consideration has to be taken into account for the alloy composition. Hence, there is still plenty of room for further understanding and optimizing ternary III-V nanowire growth for device applications. This section gives an overview of the existing knowledge on growth and characteristic properties of ternary III-V nanowires focusing on InxGa1-xAs nanowires including recent development of InxGa1-xAs
nanowire device applications.
1.2.1 Growth of ternary III-V nanowires
As with other semiconductor nanowires, ternary III-V semiconductor nanowires can be grown via the common nanowire growth methods such as vapour-liquid-solid (VLS) (foreign metal seed or self-seeded) and direct (particle-free) vapour-solid (VS) growth through methods such as selected-area epitaxy (SAE). These basic concepts of the growth methods will be further discussed in chapter 2. In this chapter, the focus is to give a review on the progress and challenges of ternary III-V nanowire growth including InxGa1-xAs
nanowires. The review is split into the two, based on their method of growth to provide the insight on the different challenges faced by each method.
18.104.22.168 VLS growth of ternary III-V nanowires
Hence it is obvious that the fundamental mechanisms of VLS growth for ternary III-V nanowires should be similar to their binaries, but more intricate due to the additional species involved.
Early VLS growths of ternary III-V nanowires include GaAsP and InAsP , InGaN , AlGaN , AlGaAs , , and InGaAs  . Growth of Au-seeded GaAsP and InAsP nanowires was considered successful using laser-assisted catalytic growth method with composition close to the given target composition . The nanowires show nearly pure zinc-blende phase and were uniform in diameter along the length of the nanowires, which exceeded 10 µm . However no composition tunability was reported in this initial growth report. On the other hand, the growth of self-catalysed InxGa1-xN via low-temperature halide
chemical vapour deposition has been shown to be successful across the entire compositional range x=0-1 by Kuykendall et al. . As indicated by the transmission electron microscopy (TEM) contrast for their InGaN nanowires, no phase segregation or any large variation of In distribution was observed. This was believed to be due to the low-temperature process and the ability for nanowires to relieve strain as compared to growth of InGaN thin films. However, their nanowires completely lacked control in terms of morphology, dimensions and growth directions.
Despite the demonstration that the global composition in a nanowire ensemble could be tuned over the full composition range, further studies on single nanowire revealed a more complex behaviour. Detailed studies of VLS grown AlGaN , AlGaAs , , InGaP , InGaAs  and GaAsP  nanowires show similar trends in terms of composition inhomogeneity along the nanowire growth axis. This inhomogeneity is believed to be due to the competitive mode of VLS growth and the vapour-solid (VS) growth on the sidewall of the nanowires , , .
Among these reports, Lim S. K. et al.  managed to control the tapering effect and minimise the inhomogeneity of the composition of Al0.16Ga0.84As by growing the nanowires
nanowires are important for many device applications and are required to allow for controlled heterostructures to be formed within the nanowires (where crossing and merging would occur for nanowires grown in random directions).
Later in 2010, Wu et al.  reported that vertical Au-seeded InGaAs nanowires can be grown on InAs (111)B substrate with reasonable uniformity within a limited length. Non-uniformity was claimed to be due to the competition of In adatoms towards the axial and the radial growths. By controlling the In diffusion area and only promoting axial growth, nanowire tapering was minimised, which in turn, resulted in better composition uniformity. They found that the diffusion area can be controlled by density of the seed particles. This is similar to the previous work shown in ref.  where InGaAs nanowires grown in high density region had better morphology with less tapering. However, this method is limited by the diffusion length of In adatoms from the substrate towards the growth front. Longer nanowires will eventually be tapered due to the insufficient diffusion length of In adatom from the substrate . Furthermore, the nanowires had stacking faults which are undesirable  and can promote more radial growth .
Aside from the composition inhomogeneity, the composition of ternary nanowires was often found to be significantly different in the nanowires than the ratio of the precursors used in the gas phase , , . For example in GaAsP nanowires, P incorporation into the nanowire via VLS is different than the expected incorporation in thin film growth which indicates that a different kinetic approach has to be taken into account in understanding the growth of ternary alloy semiconductor nanowires grown by the VLS method . Growth of InAsSb also shows that incorporation of Sb radially differs from the VLS grown core . In other cases, limitation of species incorporation into solid nanowire were reported , . This in turn limits the composition tunability of the alloy composition. For instance, in Ga-assisted growth of InGaAs nanowires, Heiss et al.  were only able to incorporate 3-5 % In into the core of their nanowires while the rest of the In are found to deposit on the sidewalls forming In-rich quantum dots. Similar findings were reported for growth of Ga-seeded InGaAs segments on GaAs nanowires where In only contributed to an increase of diameter but was insufficient to incorporate into the nanowire core . On the other hand,Guo et al.  reported that InGaAs nanowires grown using Au seed had to surpass a certain In threshold in the Au alloy to be incorporated into the nanowire.
was claimed that the phase of the Au-alloy might change with temperature and in their case, Ga was found to be more thermodynamically favoured in the Au-alloy at higher temperatures (>450 ºC) leading to more Ga incorporated into the nanowires. Hence, the role of Au is much more critical in ternary nanowires as it can determine their final composition. Therefore it is essential to gain more knowledge of the growth mechanism of Au seeded ternary nanowires.
The presence and the amount of an additional species can affect the composition of the alloy particle which in turn changes the nucleation energy at the interface of Au particle-nanowire, thus affecting the nanowire crystal phase and morphology . The interplay between the alloy composition and nucleation energy can also be observed in the growth of axial heterostructures involving ternary alloys where an additional species is introduced to a binary stem such as in growth of Au-seeded InGaAs on GaAs . In such system, the heterointerfaces indicates that there is a significant difference in between different interfaces (ie; InAs/InGaAs and InGaAs/InAs interface) indicating that the VLS method is sensitive to change in composition and indicates that In can be residual in the Au alloy even after In supply is ended. In the case where tunability of alloy composition was achieved (InGaAs and GaAsP nanowires ) , , the crystal phase was shown to be affected by the composition, although no clear trend was observed.
From these reports, it is clear that the composition plays a large role in controlling the crystal phase, which result from the change at the alloy particle-nanowire interface. However no clear understanding is yet presented for such a trend. These trends clearly indicate that alloying phase and composition of the seed particle is highly important and solubility of individual species may affect the final nanowire composition when growing ternary nanowires.
Other than the composition inhomogeneity caused by the competition between VLS and VS growth modes, there are also reports on segregation of species in certain facets in ternary nanowires leading to inhomogeneity of composition across the nanowire. For example, As-rich bands in the corner of the side facets has been observed in GaAsSb , . Other ternary nanowires such as InGaAs and GaAsP also show In-rich and P-rich bands in the <112> direction respectively , . Similar type of segregation has also been previously observed in AlxIn1-XP shell , , AlGaAs shell nanowires – and more
spontaneously formed segregation can be beneficial in designing the quantum confinement region within a nanowire .
Overall from these reports, VLS ternary III-V nanowires including InGaAs are yet to be optimised for simultaneously achieving composition homogeneity, crystal phase
purity and desirable untapered vertical morphology suitable for device applications.
Correlation between crystal phase and composition has been presented and remains as an interesting area to be explored. Such observation can provide more knowledge on the limitation and interplay between the composition and crystal phase of VLS nanowires. The growth of VLS ternary III-V nanowires is certainly complex, particularly when involving other metals such as Au. Understanding the growth mechanism behind all these observations is required to control the growth of ternary nanowires with desired properties.
22.214.171.124 Particle/droplet free growth of InGaAs nanowires
Apart from VLS growth, ternary III-V nanowires can also be grown without the apparent use of a droplet. Self-assembled growth of InxGa1-xAs nanowires grown on Si reported by Shin et al.  show composition inhomogeneity despite of being taper-free. The inhomogeneity was indicated by the strain related bending their nanowires. The composition was also found to be related to the crystal phase where In-rich InGaAs had a higher density of ZB segments than the Ga-rich InGaAs. However over the wide range of composition reported, nanowires are highly defective . On the other hand, pure WZ phase micro-sized InGaAs pillars were reported with high composition uniformity as shown by EDX mapping of the pillars , . However these large cone-shape pillars and the low density could limit their application in devices.
Growth of InGaAs nanowires on graphene were successfully demonstrated using van der Waals epitaxy . However the nanowires spontaneously formed a core-shell structure with InAs core and InGaAs shell. The core-shell structure was elucidated due to the use of graphene substrate, where InAs core was formed as its lattice parameter was nearly matched to that of the graphene substrate.
uniform arrays contributing to a more uniform composition of InGaAs among the nanowires. However these nanowires grown by particle-free SAE methods still suffer from a high density of stacking faults –.
From the limited amount of particle-free growth of ternary InGaAs nanowires, it can be concluded that these nanowires can be obtained with uniform composition far more easily due to the absence of a metal seed which creates anisotropy in adatom incorporation. However this growth method still faces severe challenges such as the lack of the crystal phase purity or the limitation in certain cases to tunability over a restricted composition range.
1.2.2 Application of ternary III-V nanowires in devices
Despite some issues in either the crystal phase or the composition, ternary III-V nanowires have already been used in some devices. Sun and Ng et al. , , have reported lasing in their InGaAs nanopillars grown on Si despite the In deficient segment within their structure. A good p-n junction was demonstrated in a photovoltaic device fabricated by Shin et al.
using InGaAs nanowires despite the polytypic crystal structure . Single GaAsP nanowire solar cell  and ternary nanowires transistors – were successfully fabricated and characterised. However, these reports do not give any structural or composition detail. Nonetheless the reported devices clearly highlight the potential of ternary nanowires.
Additionally, nanowire devices incorporating heterostructures containing ternary alloy materials have also been demonstrated as light emitters from InGaAs quantum dots embedded in GaAs nanowires ; InGaN multi quantum well laser , solar cells with InGaAs/GaAs axial junction  and InGaAs/GaAsP/GaAs LEDs .
1.2.3 Ternary III-V nanowires review summary
In summary, the brief review of the growth of ternary group III-V has been presented. Ternary III-V nanowires are challenging due to the composition inhomogeneity of the alloy within the nanowire. Despite some of the reported composition homogeneity, there are still some issues such as defects, crystal phase control, tapering, and time dependent limitation as presented briefly in this chapter. Hence, this thesis is devoted towards understanding the growth of one ternary alloy III-V semiconductor, InGaAs. The objective is to gain in-depth knowledge of how Au-seeded InGaAs nanowires grow under different growth conditions and how to control the growth and properties of these Au-seeded InGaAs nanowires to simultaneously achieve desired morphological, crystal phase and composition homogeneity. Composition tunability and the effect of composition on the crystal structure are two other interesting areas to be further understood in order to be able to control growth of ternary nanowires. By having control of the composition of ternary nanowires and their structural properties, more complex heterostructures and devices can be realised with improved performance.
1.3 Thesis synopsis
This thesis is divided into 8 chapters.
The first (current) introduction chapter includes the basics of InGaAs as a semiconductor material, a brief review of ternary III-V nanowires and introduces the global aims of this thesis. This chapter also highlights the areas which require attention which could be enhanced further to improve our knowledge in understanding the growth mechanism of ternary alloy nanowires, especially InGaAs nanowires which has great potential in high-speed telecommunication and near infra-red application.
Chapter 2 discusses the basic concepts of semiconductor nanowires, growth of nanowires and their heterostructures and their crystallographic structural properties.
In chapter 4, the results obtained via two-temperature growth method are discussed. Although the two-temperature growth technique has been a great a success to synthesise high quality GaAs nanowires, it is more challenging in growing ternary InGaAs nanowires which results in further complexity. This chapter discusses the effect of growth temperature, precursor ratios and vapour composition. Albeit challenging, successful InGaAs nanowires with pure ZB phase could be achieved for high In content (In0.95Ga0.05As).
Such nanowires are useful to replace InAs nanowires as they have lower leakage current due to the larger bandgap with the introduction of Ga. Hence, it is highly important to be able to grow such structures with highly pure crystal phase in order to realise fast-switching devices which require high electron mobility.
In chapter 5, growth of InGaAs nanowires aiming at a uniform pure WZ crystal structure and high compositional homogeneity is presented. V/III ratio is shown to have control over the tunability of InGaAs composition and crystal phase. The key factors for achieving uniform composition are summarised. In0.65Ga0.35As nanowires are shown to grow
with negligible tapering, uniform composition and were shown to have strong emission at the desirable wavelength for telecommunications applications around 1.55 µm when capped with an InP shell.
A growth model is then proposed and developed to further understand the growth trend observed as detailed in chapter 6. The main factors affecting the axial growth rate and the composition of InGaAs nanowires are extracted based on correlation of the model to the experimental results. The model provides a better understanding on the growth of InGaAs nanowires.
Chapter 7 shows and discusses the results of InGaAs/InGaP core-shell heterostructures. It explores tuning of the bandgap of the InGaAs core using various shell thickness. The chapter also discusses the growth of InGaP shell on WZ phase InGaAs and ZB InGaAs nanowires. The bandgap of InGaAs nanowires is shown to be tunable using InGaP shell with various shell thicknesses.
 R. S. Wagner and W. C. Ellis, “Vapor-liquid-solid mechanism of single crystal growth,”
Appl. Phys. Lett., vol. 4, no. 5, pp. 89–90, 1964.
 E. I. Givargizov, “Fundamental aspects of VLS growth,” J. Cryst. Growth, vol. 31, pp. 20– 30, 1975.
 K. A. Dick, “A review of nanowire growth promoted by alloys and non-alloying
elements with emphasis on Au-assisted III-V nanowires,” Prog. Cryst. Growth Charact. Mater., vol. 54, no. 3–4, pp. 138–173, 2008.
 S. A. Fortuna and X. Li, “Metal-catalyzed semiconductor nanowires: a review on the control of growth directions,” Semicond. Sci. Technol., vol. 25, no. 2, p. 024005, 2010.
 R. R. Lapierre, A. C. E. Chia, S. J. Gibson, C. M. Haapamaki, J. Boulanger, R. Yee, P. Kuyanov, J. Zhang, N. Tajik, N. Jewell, and K. M. A. Rahman, “III-V nanowire
photovoltaics: Review of design for high efficiency,” Phys. Status Solidi - Rapid Res. Lett., vol. 7, no. 10, pp. 815–830, 2013.
 L. Vj, J. Oh, A. P. Nayak, A. M. Katzenmeyer, K. Gilchrist, S. Grego, N. P. Kobayashi, S. Wang, A. A. Talin, N. K. Dhar, and M. M. Islam, “A Perspective on Nanowire
Photodetectors: Current Status, Future Challenges, and Opportunities,” Sel. Top. Quantum Electron. IEEE J., vol. PP, no. 99, pp. 1–31, 2011.
 C. Soci, A. Zhang, X.-Y. Bao, H. Kim, Y. Lo, and D. Wang, “Nanowire photodetectors.,” J. Nanosci. Nanotechnol., vol. 10, no. 3, pp. 1430–1449, 2010.
 E. C. Garnett, M. L. Brongersma, Y. Cui, and M. D. McGehee, “Nanowire Solar Cells,”
Annu. Rev. Mater. Res., vol. 41, no. 1, pp. 269–295, 2011.
 S. Barth, F. Hernandez-Ramirez, J. D. Holmes, and A. Romano-Rodriguez, “Synthesis and applications of one-dimensional semiconductors,” Prog. Mater. Sci., vol. 55, no. 6, pp. 563–627, 2010.
 X. Zhuang, C. Z. Ning, and A. Pan, “Composition and bandgap-graded semiconductor alloy nanowires,” Adv. Mater., vol. 24, no. 1, pp. 13–33, 2012.
 L.-E. Wernersson, C. Thelander, E. Lind, and L. Samuelson, “III-V Nanowires - Extending a Narrowing Road,” Proc. IEEE, vol. 98, no. 12, pp. 2047–2060, 2010.
 A. Rogalski and K. Chrzanowski, “Infrared devices and techniques,” Optoelectron. Rev., vol. 10, no. 2, pp. 653–691, 2002.
 R. E. Nahory, M. A. Pollack, W. D. Johnston, and R. L. Barns, “Band gap versus
composition and demonstration of Vegard’s law for In1−xGaxAsyP1−y lattice matched to
InP,” Appl. Phys. Lett., vol. 33, no. 7, p. 659, Aug. 1978.
 Y. Li, F. Qian, J. Xiang, and C. M. Lieber, “Nanowire electronic and optoelectronic devices Electronic and optoelectronic devices impact many areas of society , from,”
Mater. Today, vol. 9, no. 10, pp. 18–27, 2006.
 H. J. Joyce, Q. Gao, H. Hoe Tan, C. Jagadish, Y. Kim, J. Zou, L. M. Smith, H. E. Jackson, J. M. Yarrison-Rice, P. Parkinson, and M. B. Johnston, “III-V semiconductor nanowires for optoelectronic device applications,” Prog. Quantum Electron., vol. 35, no. 2–3, pp. 23– 75, 2011.
 J. W. Harrison and J. R. Hauser, “Alloy scattering in ternary III-V compounds,” Phys. Rev. B, vol. 13, no. 12, 1976.
 M. Ichimura and A. Sasaki, “Short-range order in III-V ternary alloy semiconductors,”
J. Appl. Phys., vol. 60, no. 11, pp. 3850–3855, 1986.
 P. Caroff, M. E. Messing, B. Mattias Borg, K. A. Dick, K. Deppert, and L.-E. Wernersson, “InSb heterostructure nanowires: MOVPE growth under extreme lattice mismatch.,”
Nanotechnology, vol. 20, no. 49, p. 495606, 2009.
 H. D. Park, S. M. Prokes, M. E. Twigg, Y. Ding, and Z. L. Wang, “Growth of high quality, epitaxial InSb nanowires,” J. Cryst. Growth, vol. 304, no. 2, pp. 399–401, Jun. 2007.
 K. A. Dick, K. Deppert, L. Samuelson, L. R. Wallenberg, and F. M. Ross, “Control of GaP and GaAs nanowire morphology through particle and substrate chemical
modification,” Nano Lett., vol. 8, no. 11, pp. 4087–4091, 2008.
 H. J. Joyce, Q. Gao, J. Wong-Leung, Y. Kim, H. H. Tan, and C. Jagadish, “Tailoring GaAs, InAs, and InGaAs nanowires for optoelectronic device applications,” IEEE J. Sel. Top. Quantum Electron., vol. 17, no. 4, pp. 766–778, 2011.
 K. A. Dick, J. Bolinsson, M. E. Messing, S. Lehmann, J. Johansson, and P. Caroff,
“Parameter space mapping of InAs nanowire crystal structure,” J. Vac. Sci. Technol. B Microelectron. Nanom. Struct., vol. 29, no. 4, p. 04D103, 2011.
 K. A. Dick, K. Deppert, L. Samuelson, and W. Seifert, “Optimization of Au-assisted InAs nanowires grown by MOVPE,” J. Cryst. Growth, vol. 297, no. 2, pp. 326–333, 2006.
 K. A. Dick, P. Caroff, J. Bolinsson, M. E. Messing, J. Johansson, K. Deppert, L. R.
Wallenberg, and L. Samuelson, “Control of III–V nanowire crystal structure by growth parameter tuning,” Semicond. Sci. Technol., vol. 25, no. 2, p. 024009, Feb. 2010.
 C. C. Chen and C. C. Yeh, “Large-scale catalytic synthesis of crystalline gallium nitride nanowires,” Adv. Mater., vol. 12, no. 10, pp. 738–741, 2000.
 K. W. Chang and J. J. Wu, “Low-temperature catalytic synthesis of gallium nitride nanowires,” J. Phys. Chem. B, vol. 106, no. 32, pp. 7796–7799, 2002.
 X. Duan and C. M. Lieber, “General synthesis of compound semiconductor nanowires,”
 T. Kuykendall, P. Ulrich, S. Aloni, and P. Yang, “Complete composition tunability of InGaN nanowires using a combinatorial approach.,” Nat. Mater., vol. 6, no. 12, pp. 951–956, 2007.
 J. Su, M. Gherasimova, G. Cui, H. Tsukamoto, J. Han, T. Onuma, M. Kurimoto, S. F. Chichibu, C. Broadbridge, Y. He, and A. V. Nurmikko, “Growth of AlGaN nanowires by metalorganic chemical vapor deposition,” Appl. Phys. Lett., vol. 87, no. 18, pp. 1–3, 2005.
 C. Chen, S. Shehata, C. Fradin, R. LaPierre, C. Couteau, and G. Weihs, “Self-directed growth of AlGaAs core-shell nanowires for visible light applications,” Nano Lett., vol. 7, no. 9, pp. 2584–2589, 2007.
 Z. H. Wu, M. Sun, X. Y. Mei, and H. E. Ruda, “Growth and photoluminescence characteristics of AlGaAs nanowires,” Appl. Phys. Lett., vol. 85, no. 4, pp. 657–659, 2004.
 Y. Kim, H. J. Joyce, Q. Gao, H. H. Tan, C. Jagadish, M. Paladugu, J. Zou, and A. A. Suvorova, “Influence of nanowire density on the shape and optical properties of ternary InGaAs nanowires,” Nano Lett., vol. 6, no. 4, pp. 599–604, 2006.
 S. K. Lim, M. J. Tambe, M. M. Brewster, and S. Gradecak, “Controlled growth of ternary alloy nanowires using metalorganic chemical vapor deposition.,” Nano Lett., vol. 8, no. 5, pp. 1386–1392, 2008.
 A. Fakhr, Y. M. Haddara, and R. R. Lapierre, “Dependence of InGaP nanowire morphology and structure on molecular beam epitaxy growth conditions.,”
Nanotechnology, vol. 21, no. 16, p. 165601, 2010.
 Y. N. Guo, H. Y. Xu, G. J. Auchterlonie, T. Burgess, H. J. Joyce, Q. Gao, H. H. Tan, C. Jagadish, H. B. Shu, X. S. Chen, W. Lu, Y. Kim, and J. Zou, “Phase separation induced by Au catalysts in ternary InGaAs nanowires,” Nano Lett., vol. 13, no. 2, pp. 643–650, 2013.
 W. Sun, Y. Huang, Y. Guo, Z. M. Liao, Q. Gao, H. H. Tan, C. Jagadish, X. Z. Liao, and J. Zou, “Spontaneous formation of core–shell GaAsP nanowires and their enhanced electrical conductivity,” J. Mater. Chem. C, vol. 3, no. 8, pp. 1745–1750, 2015.
 J. Wu, B. M. Borg, D. Jacobsson, K. A. Dick, and L. E. Wernersson, “Control of composition and morphology in InGaAs nanowires grown by metalorganic vapor phase epitaxy,” J. Cryst. Growth, vol. 383, pp. 158–165, 2013.
 C. Thelander, P. Caroff, S. Plissard, A. W. Dey, and K. A. Dick, “Effects of crystal phase mixing on the electrical properties of InAs nanowires,” Nano Lett., vol. 11, no. 6, pp. 2424–2429, 2011.
 P. J. Poole, D. Dalacu, X. Wu, J. Lapointe, and K. Mnaymneh, “Interplay between crystal phase purity and radial growth in InP nanowires,” Nanotechnology, vol. 23, no. 38, p. 385205, 2012.
 Y. Y. Zhang, M. Aagesen, J. V Holm, H. I. Jorgensen, J. Wu, and H. Y. Liu, “Self-Catalyzed GaAsP Nanowires Grown on Silicon Substrates by Solid-Source Molecular Beam Epitaxy,” Nano Lett., vol. 13, pp. 3897–3902, 2013.
 T. Xu, K. A. Dick, S. Plissard, T. H. Nguyen, Y. Makoudi, M. Berthe, J.-P. Nys, X. Wallart, B. Grandidier, and P. Caroff, “Faceting, composition and crystal phase evolution in III– V antimonide nanowire heterostructures revealed by combining microscopy
techniques,” Nanotechnology, vol. 23, no. 9, p. 095702, 2012.
 M. Heiss, A. Gustafsson, S. Conesa-Boj, F. Peiró, J. R. Morante, G. Abstreiter, J. Arbiol, L. Samuelson, and A. Fontcuberta i Morral, “Catalyst-free nanowires with axial InxGa1-xAs/GaAs heterostructures.,” Nanotechnology, vol. 20, no. 7, p. 075603, 2009.
 J. Paek, M. Yamaguchi, and H. Amano, “MBE-VLS growth of catalyst-free III-V axial heterostructure nanowires on (1 1 1)Si substrates,” J. Cryst. Growth, vol. 323, no. 1, pp. 315–318, 2011.
 S. G. Ghalamestani, M. Ek, M. Ghasemi, P. Caroff, J. Johansson, and K. A. Dick, “Morphology and composition controlled GaxIn1-xSb nanowires: understanding
ternary antimonide growth.,” Nanoscale, vol. 6, no. 2, pp. 1086–92, 2014.
 J. Bauer, V. Gottschalch, H. Paetzelt, and G. Wagner, “VLS growth of
GaAs/(InGa)As/GaAs axial double-heterostructure nanowires by MOVPE,” J. Cryst. Growth, vol. 310, no. 23, pp. 5106–5110, 2008.
 C. S. Jung, H. S. Kim, G. B. Jung, K. J. Gong, Y. J. Cho, S. Y. Jang, C. H. Kim, C. W. Lee, and J. Park, “Composition and phase tuned InGaAs alloy nanowires,” J. Phys. Chem. C, vol. 115, no. 16, pp. 7843–7850, 2011.
 H. S. Im, C. S. Jung, K. Park, D. M. Jang, Y. R. Lim, and J. Park, “Band gap tuning of twinned GaAsP ternary nanowires,” J. Phys. Chem. C, vol. 118, no. 8, pp. 4546–4552, 2014.
 S. Conesa-Boj, D. Kriegner, X. L. Han, S. Plissard, X. Wallart, J. Stangl, A. Fontcuberta I Morral, and P. Caroff, “Gold-free ternary III-V antimonide nanowire arrays on silicon: Twin-free down to the first bilayer,” Nano Lett., vol. 14, no. 1, pp. 326–332, 2014.
 X. Yuan, P. Caroff, J. Wong-Leung, H. H. Tan, and C. Jagadish, “Controlling the morphology, composition and crystal structure in gold-seeded GaAs 1−x Sb x nanowires,” Nanoscale, vol. 7, no. 11, pp. 4995–5003, 2015.
 Y. N. Guo, T. Burgess, Q. Gao, H. H. Tan, C. Jagadish, and J. Zou, “Polarity-driven nonuniform composition in InGaAs nanowires,” Nano Lett., vol. 13, no. 11, pp. 5085– 5089, 2013.
 N. Sköld, J. B. Wagner, G. Karlsson, T. Hernán, W. Seifert, M.-E. Pistol, and L.
Samuelson, “Phase segregation in AlInP shells on GaAs nanowires.,” Nano Lett., vol. 6, no. 12, pp. 2743–2747, 2006.
 J. B. Wagner, N. Sköld, L. Reine Wallenberg, and L. Samuelson, “Growth and
 N. Jiang, Q. Gao, P. Parkinson, J. Wong-Leung, S. Mokkapati, S. Breuer, H. H. Tan, C. L. Zheng, J. Etheridge, and C. Jagadish, “Enhanced minority carrier lifetimes in
GaAs/AlGaAs core-shell nanowires through shell growth optimization,” Nano Lett., vol. 13, no. 11, pp. 5135–5140, 2013.
 M. Fickenscher, T. Shi, H. E. Jackson, L. M. Smith, J. M. Yarrison-rice, C. Zheng, P. Miller, J. Etheridge, B. M. Wong, Q. Gao, S. Deshpande, H. H. Tan, and C. Jagadish, “Optical , Structural , and Numerical Investigations of GaAs / AlGaAs Core − Multishell Nanowire Quantum Well Tubes,” 2013.
 D. Rudolph, S. Funk, M. Döblinger, S. Morkötter, S. Hertenberger, L. Schweickert, J. Becker, S. Matich, M. Bichler, D. Spirkoska, I. Zardo, J. J. Finley, G. Abstreiter, and G. Koblmüller, “Spontaneous alloy composition ordering in GaAs-AlGaAs core-shell nanowires,” Nano Lett., vol. 13, no. 4, pp. 1522–1527, 2013.
 H. Kauko, C. L. Zheng, Y. Zhu, S. Glanvill, C. Dwyer, A. M. Munshi, B. O. Fimland, A. T. J. Van Helvoort, and J. Etheridge, “Compositional analysis of GaAs/AlGaAs
heterostructures using quantitative scanning transmission electron microscopy,”
Appl. Phys. Lett., vol. 103, no. 23, 2013.
 Y. Zhang, A. M. Sanchez, J. Wu, M. Aagesen, J. V. Holm, R. Beanland, T. Ward, and H. Liu, “Polarity-Driven Quasi-3-Fold Composition Symmetry of Self-Catalyzed III–V–V Ternary Core–Shell Nanowires,” Nano Lett., vol. 15, pp. 3128–3133, 2015.
 M. Heiss, Y. Fontana, A. Gustafsson, G. Wüst, C. Magen, D. D. O’Regan, J. W. Luo, B. Ketterer, S. Conesa-Boj, A. V Kuhlmann, J. Houel, E. Russo-Averchi, J. R. Morante, M. Cantoni, N. Marzari, J. Arbiol, A. Zunger, R. J. Warburton, and A. Fontcuberta i Morral, “Self-assembled quantum dots in a nanowire system for quantum photonics.,” Nat. Mater., vol. 12, no. 5, pp. 439–44, 2013.
 J. C. Shin, K. H. Kim, K. J. Yu, H. Hu, L. Yin, C. Ning, J. a Rogers, J. Zuo, and X. Li, “In
xGa1 - xAs Nanowires on Silicon : One-Dimensional Heterogeneous epitaxy, bandgap
engineering and photovotaic,” Nano Lett., vol. 11, pp. 4831–4838, 2011.
 K. W. Ng, W. S. Ko, F. Lu, and C. J. Chang-Hasnain, “Metastable growth of pure wurtzite InGaAs microstructures,” Nano Lett., vol. 14, no. 8, pp. 4757–4762, 2014.
 K. W. Ng, W. S. Ko, R. Chen, F. Lu, T. D. Tran, K. Li, and C. J. Chang-Hasnain,
“Composition Homogeneity in InGaAs/GaAs Core − Shell Nanopillars Monolithically Grown on Silicon,” Appl. Mater. Interfaces, vol. 6, no. 19, pp. 16706–11, 2014.
 P. K. Mohseni, A. Behnam, J. D. Wood, C. D. English, J. W. Lyding, E. Pop, and X. Li, “InxGa1-xAs Nanowire Growth on Graphene: van der Waals Epitaxy Induced Phase
Segregation,” Nano Lett., vol. 13, pp. 1153–1161, 2013.
 Y. Kohashi, T. Sato, K. Ikejiri, K. Tomioka, S. Hara, and J. Motohisa, “Influence of growth temperature on growth of InGaAs nanowires in selective-area metalorganic vapor-phase epitaxy,” J. Cryst. Growth, vol. 338, no. 1, pp. 47–51, 2012.
 T. Sato, J. Motohisa, J. Noborisaka, S. Hara, and T. Fukui, “Growth of InGaAs nanowires by selective-area metalorganic vapor phase epitaxy,” J. Cryst. Growth, vol. 310, no. 7– 9, pp. 2359–2364, 2008.
 M. Yoshimura, K. Tomioka, K. Hiruma, S. Hara, J. Motohisa, and T. Fukui, “Growth and characterization of InGaAs nanowires formed on GaAs(111)B by selective-area metal organic vapor phase epitaxy,” Jpn. J. Appl. Phys., vol. 49, no. 4 PART 2, pp. 8–12, 2010.
 S. Hertenberger, S. Funk, K. Vizbaras, a. Yadav, D. Rudolph, J. Becker, S. Bolte, M. Döblinger, M. Bichler, G. Scarpa, P. Lugli, I. Zardo, J. J. Finley, M. C. Amann, G. Abstreiter, and G. Koblmüller, “High compositional homogeneity in In-rich InGaAs nanowire arrays on nanoimprinted SiO 2/Si (111),” Appl. Phys. Lett., vol. 101, no. 4, 2012.
 G. Koblmuller and G. Abstreiter, “Growth and properties of InGaAs nanowires on silicon,” Phys. Status Solidi RRL, vol. 7, no. 10, pp. 1–20, 2014.
 H. Sun, F. Ren, K. W. Ng, T. T. D. Tran, K. Li, and C. J. Chang-Hasnain, “Nanopillar lasers directly grown on silicon with heterostructure surface passivation,” ACS Nano, vol. 8, no. 7, pp. 6833–6839, 2014.
 J. V Holm, H. I. Jørgensen, P. Krogstrup, J. Nygård, H. Liu, and M. Aagesen, “Surface-passivated GaAsP single-nanowire solar cells exceeding 10% efficiency grown on silicon.,” Nat. Commun., vol. 4, p. 1498, 2013.
 T. Yang, S. Hertenberger, S. Morkötter, G. Abstreiter, and G. Koblmüller, “Size, composition, and doping effects on In(Ga)As nanowire/Si tunnel diodes probed by conductive atomic force microscopy,” Appl. Phys. Lett., vol. 101, no. 23, pp. 233102–1– 5, 2012.
 J. J. Hou, N. Han, F. Wang, F. Xiu, S. Yip, A. T. Hui, T. Hung, and J. C. Ho, “Synthesis and characterizations of ternary InGaAs nanowires by a two-step growth method for high-performance electronic devices,” ACS Nano, vol. 6, no. 4, pp. 3624–3630, 2012.
 K. Tomioka, M. Yoshimura, and T. Fukui, “A III–V nanowire channel on silicon for high-performance vertical transistors,” Nature, vol. 488, no. 7410, pp. 189–192, 2012.
 M. N. Makhonin, a. P. Foster, a. B. Krysa, P. W. Fry, D. G. Davies, T. Grange, T. Walther, M. S. Skolnick, and L. R. Wilson, “Homogeneous array of nanowire-embedded
quantum light emitters,” Nano Lett., vol. 13, no. 3, pp. 861–865, 2013.
 F. Qian, Y. Li, S. Gradecak, H.-G. Park, Y. Dong, Y. Ding, Z. L. Wang, and C. M. Lieber, “Multi-quantum-well nanowire heterostructures for wavelength-controlled lasers.,”
Nat. Mater., vol. 7, no. 9, pp. 701–706, 2008.
 E. Nakai, M. Chen, M. Yoshimura, K. Tomioka, and T. Fukui, “InGaAs axial-junction nanowire-array solar cells,” Jpn. J. Appl. Phys., vol. 54, p. 015201, 2015.
This chapter introduces the general concepts used throughout the thesis. It specifically focuses on semiconductor nanowire growth principles and their structural properties. These concepts make up the foundation for the interpretation and discussion of results presented in chapters 4 to 7. Sections 2.1 to 2.3 briefly introduce semiconductor nanowires, their heterostructures and applications. This is followed by nanowire growth concepts in section 2.4, focusing exclusively on metal seeded nanowire growth via vapour-liquid-solid (VLS) mechanism. This section also includes the challenges faced in growing nanowire heterostructures by VLS. The chapter then continues with III-V nanowire crystal structure including a brief discussion of crystal phase control reported for III-V Au seeded nanowires.
2.1 Semiconductor nanowires
counterparts. For example, the small diameter allows for quantum confinement in the 1-D direction, thereby enabling the tuning of the optical and electrical properties with diameters –. The large surface area of nanowires and proximity of the surface to the core make them sensitive to changes on the surface thus making them suitable for applications such as chemical/biological sensors  and gas detectors . Additionally, their large surface-to-volume ratio also enables effective strain release which is an advantage for various heterostructures required for semiconductor devices . Furthermore, their geometry also makes them great optical cavities, perfect for making tiny lasers –. This is highly promising for integration with nanoscale electronics enabling smaller, yet more functional devices for the future.
Another advantage of nanowires is the ability to grow in different crystal phase unlike bulk semiconductors. For example, many III-V nanowires can grow in the wurtzite (WZ) phase whereas in the bulk form they exist as zinc-blende (ZB) phase. WZ and ZB crystal phases have different bandstructures, which can provide another avenue for tunability. This shall be further discussed in section 2.4.
Due to these interesting properties, nanowires offer many opportunities for building nanoscale electronic and optoelectronic devices. In the electronics field, nanowire transistors have been realized – which shows the potential in further reducing the size of electronic chips and increasing the speed of devices. Multi-colour lasers , light emitting diodes (LED) –, solar cells – and photodetectors ,  are some other optical devices that have been demonstrated with nanowires. Furthermore, nanowires show the prospect for water splitting applications  and self-powering sensors . Nanowires are also suitable for energy conversion other than solar cells such as electrochemical energy storage and thermoelectric applications , . Other potential nanowire applications also include bio-applications such as single cell endoscopy .